International Journal of Metals

Volume 2014, Article ID 286393, 7 pages

http://dx.doi.org/10.1155/2014/286393

## Band Gap Engineering of Alloys

^{1}Laboratory of Physical Chemistry of Advanced Materials, University of Djillali Liabes, BP 89, 22000 Sidi Bel Abbes, Algeria^{2}Physics Department, Science Faculty, University of Sidi Bel Abbes, 22000 Sidi Bel Abbes, Algeria

Received 13 August 2013; Revised 3 February 2014; Accepted 2 March 2014; Published 13 May 2014

Academic Editor: Velimir Radmilovic

Copyright © 2014 Djillali Bensaid et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

The structural and electronic properties of the ternary alloys have been calculated using the full-potential linear muffin-tin-orbital (FP-LMTO) method based on density functional theory within local density approximation (LDA). The calculated equilibrium lattice constants and bulk moduli are compared with previous results. The concentration dependence of the electronic band structure and the direct and indirect band gaps are investigated. Moreover, the refractive index and the optical dielectric constant for are studied. The thermodynamic stability of the alloys of interest is investigated by means of the miscibility. This is the first quantitative theoretical prediction to investigate the effective masses, optical and thermodynamic properties for alloy, and still awaits experimental.

#### 1. Introduction

In recent years, the wide-gap II–VI compounds are widely investigated because of the attractive applications in fabricating blue-green and blue optoelectronic devices, such as light-emitting diodes and laser diodes [1–4]. The applications include the use of II–VI compound based materials as light sources, in full colour displays, and for increasing the information density in optical recording [5, 6]. The beryllium containing II–VI compounds had been found to possess an enhanced ability to significantly reduce the defect propagation due to a greater prevalence of strong covalent bonding and lattice hardening in the materials [7, 8]. The strong covalent bonding in beryllium-based II–VI compounds achieves a considerable lattice hardening, which avoids multiplication of defects during the operation of II–VI semiconductor laser devices [9, 10] alloys have attracted great attention because they are promising for the fabrication of full-colour visible optical devices due to a large difference in the energy gaps of the binary constituents (CdSe, eV; BeSe, eV) [11].

In the present theoretical work, band gap of zinc-blende CdSe is varied systematically by alloying with Be. In order to investigate the optoelectronic nature of these alloys, their structural, electronic, and optical properties are calculated. All calculations are based on density functional full-potential linear muffin-tin orbital (FP-LMTO) method with perdew-wang local density approximation (LDA).

#### 2. Method of Calculations

The calculations reported here were carried out using the* ab initio* full-potential linear muffin-tin orbital (FP-LMTO) method [12–15] as implemented in the Lmtart code [16]. The exchange and correlation potential was calculated using the local density approximation (LDA) [17]. The FP-LMTO is an improved method compared to previous LMTO techniques, and it treats muffin-tin spheres and interstitial regions on the same footing, leading to improvements in the precision of the eigenvalues. At the same time, the FP-LMTO method, in which the space is divided into an interstitial region (IR) and nonoverlapping muffin-tin spheres (MTS) surrounding the atomic sites, uses a more complete basis than its predecessors. In the IR regions, the basis set consists of plane waves. Inside the MT spheres, the basis set is described by radial solutions of the one particle Schrödinger equation (at fixed energy) and their energy derivatives multiplied by spherical harmonics. The charge density and the potential are represented inside the MTS by spherical harmonics up to . The integrals over the Brillouin zone are performed up to 35 special -points for binary compounds and 27 special points for the alloys in the irreducible Brillouin zone (IBZ) using Blochl’s modified tetrahedron method [18]. The self-consistent calculations are considered to be converged when the total energy of the system is stable within 10^{−6} Ry. In order to avoid the overlap of atomic spheres, the MTS radius for each atomic position is taken to be different for each composition. We point out that the use of the full-potential calculation ensures that the calculation is not completely independent of the choice of sphere radii.

Structural properties of are calculated using Murnaghan’s equation of state [19] as follows: where is the total energy of the supercell, is the unit volume, is the bulk modulus at zero pressure, and is the derivative of bulk modulus with pressure.

Optical properties of are calculated using a fine mesh of 1500 points for the present calculation. The dielectric function of a crystal depends on the electronic band structure and its investigation by optical spectroscopy which is a powerful tool in the determination of the overall optical behavior of a compound. It can be divided into two parts, real and imaginary as follows: The imaginary part of the complex dielectric function, , in cubic symmetry compounds can be calculated by the following relation [20, 21]: while is used to calculate the real part of the complex dielectric function as follows: Refractive index is calculated in terms of real and imaginary parts of dielectric function by the following relation

#### 3. Result and Discussion

In order to study the structural properties of , alloys are modeled at various compositions of Be with a step of 0.25. Structure optimization of each compound is performed by minimizing the total energy with respect to the unit cell volume and ratio using Murnaghan’s equation of state [19]. The crystal structure of CdSe and BeSe zinc-blende with space group (no. 216). Structural parameters such as lattice constant, (Å), are calculated from the stable volume and are presented in Table 1. It is clear from the table that our calculated results for the binary compounds are in good agreement with the available experimental and calculated data.

Figures 1 and 2 show the variation of the calculated equilibrium lattice constant and bulk modulus as a function of concentrations for the alloy. The obtained results for the composition dependence of the calculated equilibrium lattice parameter almost follow Vegard’s law [22]. In going from CdSe to BeSe, when the Be-content increases, the values of the lattice parameters of the alloy decrease. This is due to the fact that the size of the Be atom is smaller than the Cd atom. On the opposite side, one can see from Figure 2 that the value of the bulk modulus increases as the Be concentration increases.

The calculated band structure and partial density of states for are presented in Figure 3. It is clear from the figure that is a direct band gap material. The substitution of Be does not affect the direct band gap nature of the compound but increases the gap, which is clear from Figure 2(d). The direct band gap varies from 0.39 to 4.45 eV and the indirect band gap also increases from 1.89 to 3.71 eV with the increase in Be concentration between 0.25 and 0.75. It is obvious from the data presented in Table 2 that our calculated values for the band gaps of CdSe and BeSe are closer to the experimental results than the other calculated ones. The reason for our better results is the use of effective Perdew and Wang potential in the LDA scheme [17] and high -points (1500). DFT always underestimates the band gaps; the origin of band structures is presented in Figure 3. In general, the band structures of these three compositions (0.25, 0.5, 0.75) are very similar. The uppermost valence band is mainly formed by Se 4p states.

The valence band maximum appears to be almost degenerate at the and points for three concentrations (0.25, 0.5, and 0.75), the energy at being (1.04, 1.29, and 1.24) eV lower than that at , respectively. On the other hand, the conduction band minimum occurs at , so there is a direct gap of 0.84, 1.44, and 2.47 eV at and an indirect – gap of 1.89, 2.74, and 3.71 eV for three concentrations (0.25, 0.5, and 0.75), respectively. To the best of our knowledge, there are no theoretical or experimental data on the energy band gaps for , 0.5, and 0.75 available in the literature to make a meaningful comparison. It is clear from the results that the conduction band is mainly composed of Be-2p state for all ternary alloys. Figures 3(a) and 3(b) show that the lower part of the valence band is composed of Cd-4d and the upper part is mainly dominated by Se-4p state. This is due to the nature of bonding. At , 0.5, and 0.75 partial covalent bond is stronger so the charge is shared by Se-4p and Be-2s states.

The calculated band gap versus concentration was fitted by a polynomial equation. The results are shown in Figure 2(d) and are summarised as follows: The variation in the band gap of provides promising results of the use of the compound in optoelectronic devices working in visible to ultraviolet regions. Depending on the need and requirement of a particular application, any desired band gap between 0.39 and 4.45 eV can be achieved.

We have calculated the frequency dependent imaginary dielectric function and real dielectric function. The effects of using points in the BZ have already been discussed in the earlier work by Khan et al. [23]. The knowledge of both the real and the imaginary parts of the dielectric function allows the calculation of important optical functions. In this work, we also present and analyse the refractive index given by (4).

The calculated imaginary part of the dielectric function for (, 0.5 and 0.75) in the energy range 0–12 eV is shown in Figure 3. It is clear from the figure that for , 0.50, 0.75, and 1.0 the critical points in the imaginary part of the dielectric function occur at about 0.85, 1.45, 2.48, and 4.45 eV, respectively. These points are closely related to the direct band gaps ; 0.84, 1.44, 2.47, and 4.45 eV of for the corresponding values of = 0. 25, 0.50, 0.75 and 1.

The calculated real parts of the complex dielectric function for are presented in Figure 3. It is clear from the figure that the static dielectric constant, , is strongly dependent on the band gap of the compound. The calculated values of for at , 0.25, 0.50, 0.75 and 1.0 are 4.35, 3.94, 3.74, 3.57, and 3.42 for corresponding direct band gaps 0.39, 0.84, 1.44, 2.47, and 4.45 eV, respectively. These data explain that the smaller energy gap yields larger value. This inverse relation of with the band gap can be explained by the Penn model [24] as follows: The calculated values of the optical dielectric constant and refractive index are listed in Table 3; comparison with the available data has been made where possible. As compared with other calculations, it seems that the values of obtained from FP-LMTO method for the end-point compounds (i.e., CdSe and BeSe) are in good agreement with the theoretical results, together with the refractive index at zero pressure. Note that is obtained from the zero-frequency limit of , and it corresponds to the electronic part of the static dielectric constant of the material, a parameter of fundamental importance in many aspects of materials properties. It is clear from Figure 4 that the refractive index of the material decreases with the increase in the Be concentration.

Figure 4 shows the variation of the computed static optical dielectric constant and static refractive index versus composition for alloys. The computed static optical dielectric constant and static refractive index versus composition were fitted by polynomial equation. The results are summarized as follows:

#### 4. Conclusions

Density functional calculations are carried out for the first time to investigate structural and optoelectronic properties . Structure as well as bonding nature of the material significantly varies with Be concentration. The lattice constant of the crystal decreases linearly with . The calculated band structure predicts that the alloys have direct band gaps, which increase with the increase in . On the basis of wide range of fundamental direct band gaps (0.39–4.45 eV) and indirect band gaps (1.89–3.71 eV) between 0.25 and 0.75, it can be concluded that the material can be used in optoelectronic devices working in the IR, visible, and UV regions of the spectrum.

#### Conflict of Interests

The authors declare that there is no conflict of interests regarding the publication of this paper.

#### References

- H. Luo and J. K. Furdyna, “The II-VI semiconductor blue-green laser: challenges and solution,”
*Semiconductor Science and Technology*, vol. 10, no. 8, p. 1041, 1995. View at Publisher · View at Google Scholar - M. C. Tamargo, W. Lin, S. P. Guo, Y. Guo, Y. Luo, and Y. C. Chen, “Full-color light-emitting diodes from ZnCdMgSe/ZnCdSe quantum well structures grown on InP substrates,”
*Journal of Crystal Growth*, vol. 214-215, pp. 1058–1063, 2000. View at Google Scholar - M. A. Haase, J. Qiu, J. M. DePuydt, and H. Cheng, “Blue-green laser diodes,”
*Applied Physics Letters*, vol. 59, no. 11, pp. 1272–1274, 1991. View at Publisher · View at Google Scholar · View at Scopus - E. Kato, H. Noguchi, M. Nagai, H. Okuyama, S. Kijima, and A. Ishibashi, “Significant progress in II-VI blue-green laser diode lifetime,”
*Electronics Letters*, vol. 34, no. 3, pp. 282–284, 1998. View at Google Scholar · View at Scopus - F. Vigué, E. Tournié, and J. P. Faurie, “Zn(Mg)BeSe-based p-i-n photodiodes operating in the blue-violet and near-ultraviolet spectral range,”
*Applied Physics Letters*, vol. 76, p. 242, 2000. View at Publisher · View at Google Scholar - V. Bousquet, E. Tournié, M. Laugt, P. Vennegues, and J. P. Faurie, “Structural and optical properties of lattice-matched ZnBeSe layers grown by molecular-beam epitaxy onto GaAs substrates,”
*Applied Physics Letters*, vol. 70, p. 3564, 1997. View at Publisher · View at Google Scholar - A. Waag, F. Fischer, K. Schüll et al., “Laser diodes based on beryllium-chalcogenides,”
*Applied Physics Letters*, vol. 70, no. 3, pp. 280–282, 1997. View at Google Scholar · View at Scopus - J. Y. Zhang, D. Z. Shen, X. W. Fan, B. J. Yang, and Z. H. Zhang, “ZnBeSe epitaxy layers grown by photo-assisted metalorganic chemical vapor deposition,”
*Journal of Crystal Growth*, vol. 214-215, pp. 100–103, 2000. View at Publisher · View at Google Scholar - A. Muñoz, P. Rodríguez-Hernández, and A. Mujica, “Ground-state properties and high-pressure phase of beryllium chalcogenides BeSe, BeTe, and BeS,”
*Physical Review B*, vol. 54, p. 11861, 1996. View at Publisher · View at Google Scholar - A. Waag, F. Fischer, H. J. Lugauer et al., “Molecular-beam epitaxy of beryllium-chalcogenide-based thin films and quantum-well structures,”
*Journal of Applied Physics*, vol. 80, no. 2, pp. 792–796, 1996. View at Google Scholar · View at Scopus - O. Maksimov, S. P. Guo, and M. C. Tamargo, “Be-Chalcogenide Alloys for Improved R-G-B LEDs: ${\text{Be}}_{x}{\text{Zn}}_{y}{\text{Cd}}_{1-x-y}\text{Se}$ on InP,”
*Physica Status Solidi B*, vol. 229, no. 2, pp. 1005–1009, 2002. View at Google Scholar - S. Y. Savrasov and D. Y. Savrasov, “Full-potential linear-muffin-tin-orbital method for calculating total energies and forces,”
*Physical Review B*, vol. 46, no. 19, pp. 12181–12195, 1992. View at Publisher · View at Google Scholar · View at Scopus - S. Y. Savrasov, “Linear-response theory and lattice dynamics: a muffin-tin-orbital approach,”
*Physical Review B*, vol. 54, p. 16470, 1996. View at Publisher · View at Google Scholar - P. Hohenberg and W. Kohn, “Inhomogeneous electron gas,”
*Physical Review B*, vol. 136, no. 3, pp. B864–B871, 1964. View at Publisher · View at Google Scholar · View at Scopus - W. Kohn and L. J. Sham, “Self-consistent equations including exchange and correlation effects,”
*Physical Review A*, vol. 140, no. 4, pp. A1133–A1138, 1965. View at Publisher · View at Google Scholar · View at Scopus - S. Y. Savrasov, “Program LMTART for electronic structure calculations,”
*Zeitschrift fur Kristallographie*, vol. 220, no. 5-6, pp. 555–557, 2005. View at Publisher · View at Google Scholar · View at Scopus - J. P. Perdew and Y. Wang, “Pair-distribution function and its coupling-constant average for the spin-polarized electron gas,”
*Physical Review B*, vol. 46, no. 20, pp. 12947–12954, 1992. View at Publisher · View at Google Scholar · View at Scopus - P. Blochl, O. Jepsen, and O. K. Andersen, “Improved tetrahedron method for Brillouin-zone integrations,”
*Physical Review B*, vol. 49, p. 16223, 1994. View at Publisher · View at Google Scholar - F. D. Murnaghan, “The compressibility of media under extreme pressures,”
*Proceedings of the National Academy of Sciences of the United States*, vol. 30, no. 9, pp. 244–247, 1944. View at Google Scholar - F. Wooten,
*Optical Properties of Solids*, Academic Press, New York, NY, USA, 1972. - M. Fox,
*Optical Properties of Solids*, Oxford University Press, 2001. - L. Vegard, “Die konstitution der mischkristalle und die raumfüllung der atome,”
*Zeitschrift für Physik*, vol. 5, no. 1, pp. 17–26, 1921. View at Publisher · View at Google Scholar · View at Scopus - M. A. Khan, A. Kashyap, A. K. Solanki, T. Nautiyal, and S. Auluck, “Interband optical properties of Ni3Al,”
*Physical Review B*, vol. 48, no. 23, pp. 16974–16978, 1993. View at Publisher · View at Google Scholar · View at Scopus - D. Penn, “Wave-number-dependent dielectric function of semiconductors,”
*Physical Review*, vol. 128, p. 2093, 1962. View at Publisher · View at Google Scholar - O. Zakharov, A. Rubio, X. Blase, M. L. Cohen, and S. G. Louie, “Quasiparticle band structures of six II-VI compounds: ZnS, ZnSe, ZnTe, CdS, CdSe, and CdTe,”
*Physical Review B*, vol. 50, no. 15, pp. 10780–10787, 1994. View at Publisher · View at Google Scholar · View at Scopus - J. Heyd, J. E. Peralta, G. E. Scuseria, and R. L. Martin, “Energy band gaps and lattice parameters evaluated with the Heyd-Scuseria-Ernzerhof screened hybrid functional,”
*The Journal of Chemical Physics*, vol. 123, p. 174101, 2005. View at Publisher · View at Google Scholar - P. Y. Yu and M. Cardona,
*Fundamentals of Semiconductors*, Springer, Berlin, Germany, 2001. - Y. H. Chang, C. H. Park, K. Sato, and H. Katayama-Yoshida, “First-principles study of the effect of the superexchange interaction in (Ga, Mn)V (
*V*= N, P, As and Sb),”*Journal of the Korean Physical Society*, vol. 49, no. 1, pp. 203–208, 2006. View at Google Scholar · View at Scopus - H. Luo, K. Ghandehari, R. G. Greene, A. L. Ruoff, S. S. Trail, and F. J. DiSalvo, “Phase transformation of BeSe and BeTe to the NiAs structure at high pressure,”
*Physical Review B*, vol. 52, p. 7058, 1995. View at Publisher · View at Google Scholar - C. Narayana, V. J. Nesamony, and A. L. Ruoff, “Phase transformation of BeS and equation-of-state studies to 96 GPa,”
*Physical Review B*, vol. 56, p. 14338, 1997. View at Publisher · View at Google Scholar - S. Laref and A. Laref, “Thermal properties of BeX (X = S, Se and Te) compounds from
*ab initio*quasi-harmonic method,”*Computational Materials Science*, vol. 51, no. 1, pp. 135–140, 2012. View at Publisher · View at Google Scholar · View at Scopus - M. Gonzalez-Diaz, P. Rodriguez-Hernandez, and A. Munoz, “Elastic constants and electronic structure of beryllium chalcogenides BeS, BeSe, and BeTefrom first-principles calculations,”
*Physical Review B*, vol. 55, p. 14043, 1997. View at Publisher · View at Google Scholar - N. Samarth, H. Luo, J. K. Furdyna et al., “Growth of cubic (zinc blende) CdSe by molecular beam epitaxy,”
*Applied Physics Letters*, vol. 54, no. 26, pp. 2680–2682, 1989. View at Publisher · View at Google Scholar · View at Scopus - I. M. Tsidilkovski,
*Band Structure of Semiconductors*, Elsevier Science & Technology Books, Amsterdam, The Netherlands, 1982. - M. Cardona, “Fundamental reflectivity spectrum of semiconductors with zinc-blende structure,”
*Journal of Applied Physics*, vol. 32, no. 10, pp. 2151–2155, 1961. View at Publisher · View at Google Scholar · View at Scopus - J. C. Salcedo-Reyes, “Electronic band structure of the ordered Zn
_{0.5}Cd_{0.5}Se alloy calculated by the semi-empirical tight-binding method considering second-nearest neighbor,”*Universitas Scientiarum*, vol. 13, no. 2, pp. 198–207. - O. Zakharov, A. Rubio, X. Blase, M. L. Cohen, and S. G. Louie, “Quasiparticle band structures of six II-VI compounds: ZnS, ZnSe, ZnTe, CdS, CdSe, and CdTe,”
*Physical Review B*, vol. 50, no. 15, pp. 10780–10787, 1994. View at Publisher · View at Google Scholar · View at Scopus - P. J. Huang, Y. S. Huang, F. Firszt et al., “Photoluminescence and contactless electroreflectance characterization of Be
_{x}Cd_{1−x}Se alloys,”*Journal of Physics: Condensed Matter*, vol. 19, no. 2, 026208 pages, 2007. View at Publisher · View at Google Scholar - S. V. Ivanov et al., in
*Abstracts of the 9th International Conference on ll-VI Compounds*, p. 209, Kyoto, Japan, 1999, (to be published in Journal of Crystal Growth, 2000). - S. V. Ivanov, O. V. Nekrutkina, V. A. Kaygorodov et al., “Optical and structural properties of BeCdSe/ZnSe QW heterostructures grown by MBE,” in
*Proceedings of the 8th Nanostructures: Physics and Technology International Symposium*, St.Petersburg, Russia, June 2000. - M. Gonzalez-Diaz, P. Rodriguez-Hernandez, and A. Munoz, “Elastic constants and electronic structure of beryllium chalcogenides BeS, BeSe, and BeTefrom first-principles calculations,”
*Physical Review B*, vol. 55, pp. 14043–14046, 1997. View at Publisher · View at Google Scholar - A. Fleszar and W. Hanke, “Electronic excitations in beryllium chalcogenides from the ab initio GW approach,”
*Physical Review B*, vol. 62, no. 4, pp. 2466–2474, 2000. View at Google Scholar · View at Scopus - W. M. Yim, J. B. Dismakes, E. J. Stofko, and R. J. Paff, “Synthesis and some properties of BeTe, BeSe and BeS,”
*Journal of Physics and Chemistry of Solids*, vol. 33, no. 2, pp. 501–505, 1972. View at Publisher · View at Google Scholar - N. A. Hamizi and M. R. Johan, “Optical properties of CdSe quantum dots via Non-TOP based route,”
*International Journal of Electrochemical Science*, vol. 7, pp. 8458–8467, 2012. View at Google Scholar - S. Ouendadji, S. Ghemid, H. Meradji, and F. E. H. Hassan, “Density functional study of ${\text{CdS}}_{1-x}{\text{Sex and CdS}}_{1-x}{\text{Te}}_{x}$
alloys,”
*Computational Materials Science*, vol. 48, no. 1, pp. 206–211, 2010. View at Publisher · View at Google Scholar · View at Scopus - T. M. Bieniewski and S. J. Czyzak, “Refractive indexes of single hexagonal ZnS and CdS crystals,”
*The Journal of the Optical Society of America*, vol. 53, no. 4, pp. 496–497, 1963. View at Publisher · View at Google Scholar - F. Kootstra, P. L. De Boeij, and J. G. Snijders, “Application of time-dependent density-functional theory to the dielectric function of various nonmetallic crystals,”
*Physical Review B*, vol. 62, p. 7071, 2000. View at Publisher · View at Google Scholar - G. P. Srivastava, H. M. Tutuncu, and N. Gunhan, “First-principles studies of structural, electronic, and dynamical properties of Be chalcogenides,”
*Physical Review B*, vol. 70, Article ID 085206, 2004. View at Publisher · View at Google Scholar - V. Wagner, J. J. Liang, R. Kruse et al., “Lattice dynamics and bond polarity of be-chalcogenides a new class of II-VI materials,”
*Physica Status Solidi B*, vol. 215, no. 1, pp. 87–91, 1999. View at Google Scholar · View at Scopus